# Investigation and Modeling of the Electrical Conductivity of Graphene Nanoplatelets-Loaded Doped-Polypyrrole

^{1}

^{2}

^{3}

^{4}

^{5}

^{*}

## Abstract

**:**

## 1. Introduction

## 2. Electrical Conductivity Models

- Aspect ratio is concerned with either shifting the percolation threshold leftward or upward; therefore, the aspect ratio can substitute the constant $a$ in the Sigmoidal equation.
- The filler roundness has an inverse relationship to the aspect ratio, as does the constant $a$ to ${x}_{o}$; in this case, the filler roundness replaced the constant ${x}_{o}$.
- The influence of surface energy on the composite is proportional to the orientation of the fillers in the matrix. This effect has an inverse impact on the electrical conductivity, as does the constant $b$. Therefore, the surface energy replaces the constant b.
- The volume fraction is taken as $x$.

## 3. Materials

^{2}/g, bulk density of 0.03–0.1 g/cm

^{3}, a diameter of 5 μm, an average thickness of 15 nm, and <1% oxygen content. The PPy has a 20 wt.% loading of carbon black. Deionized water was used for the experiment.

## 4. Processing of Polymer Composites

#### The Electrical Conductivity Measurement

## 5. Results and Discussion

#### 5.1. Morphology Analysis of the Hybrids

#### 5.2. Thermal Analysis of the Hybrids

#### 5.3. Structural Characterization

#### 5.4. HGPPy.CB_{20%} Electrical Conductivity

^{−3}S/m and 552 S/m, respectively. The electrical conductivity measurements for the $\mathrm{HGPPy}.{\mathrm{CB}}_{20\%}$ can be found in Figure 9. As shown in Figure 9, the electrical characteristics of the $\mathrm{HGPPy}.{\mathrm{CB}}_{20\%}$ changes as the weight fraction of the Gr changes. At Gr weight fraction of 0.15 wt.%, the hybrid begins continuous conduction, which connotes the percolation network formation. In other words, the percolation threshold of the hybrid occurred at 0.15 wt.%. At this point, there is a linear increment in the system’s electrical conductivity until 0.25 wt.%, when the hybrid begins to saturate. These results confirm the effectiveness and ability of Gr to improve polymers’ electrical conductivity at low or moderate quantity for diverse applications [32,55,56,57]. This, of course, can be attributed to the homogenous dispersion of Gr onto the $\mathrm{PPy}.{\mathrm{CB}}_{20\%}$ matrix and the ability of Gr to link the carrier transport through the van der Waals force and the $\pi -\pi $ interactions exemplified by the materials [33,46].

#### 5.5. Measurement and Model Comparison

## 6. Conclusions

## Author Contributions

## Funding

## Data Availability Statement

## Acknowledgments

## Conflicts of Interest

## References

- Le, T.-H.; Kim, Y.; Yoon, H. Electrical and electrochemical properties of conducting polymers. Polymers
**2017**, 9, 150. [Google Scholar] [CrossRef] [PubMed] - Villanueva, R.; Ganta, D.; Guzman, C. Mechanical, in-situ electrical and thermal properties of wearable conductive textile yarn coated with polypyrrole/carbon black composite. Mater. Res. Express
**2018**, 6, 016307. [Google Scholar] [CrossRef] - Yang, C.; Liu, P.; Wang, T. Well-Defined core−shell carbon black/polypyrrole nanocomposites for electrochemical energy storage. ACS Appl. Mater. Interfaces
**2011**, 3, 1109–1114. [Google Scholar] [CrossRef] [PubMed] - Yuan, Y.; Kim, S.-H. Improved performance of a microbial fuel cell with polypyrrole/carbon black composite coated carbon paper anodes. Bull. Korean Chem. Soc.
**2008**, 29, 1344–1348. [Google Scholar] - Georgakilas, V.; Perman, J.A.; Tucek, J.; Zboril, R. Broad family of carbon nanoallotropes: Classification, chemistry, and applications of fullerenes, carbon dots, nanotubes, graphene, nanodiamonds, and combined superstructures. Chem. Rev.
**2015**, 115, 4744–4822. [Google Scholar] [CrossRef] - Liu, M.-S.; Lin, M.C.-C.; Huang, I.-T.; Wang, C.-C. Enhancement of thermal conductivity with carbon nanotube for nanofluids. Int. Commun. Heat Mass Transf.
**2005**, 32, 1202–1210. [Google Scholar] [CrossRef] - Bianco, A.; Cheng, H.-M.; Enoki, T.; Gogotsi, Y.; Hurt, R.H.; Koratkar, N.; Kyotani, T.; Monthioux, M.; Park, C.R.; Tascon, J.M.; et al. All in the graphene family—A recommended nomenclature for two-dimensional carbon materials. Carbon
**2013**, 65, 1–6. [Google Scholar] [CrossRef] - Wick, P.; Louw-Gaume, A.E.; Kucki, M.; Krug, H.F.; Kostarelos, K.; Fadeel, B.; Dawson, K.A.; Salvati, A.; Vázquez, E.; Ballerini, L.; et al. Classification framework for graphene-based materials. Angew. Chem. Int. Ed.
**2014**, 53, 7714–7718. [Google Scholar] [CrossRef] [Green Version] - Kumar, V.; Monika; Lee, D.-J. High-actuation displacement with high flexibility for silicone rubber and few layer graphene composites. Sens. Actuators A Phys.
**2020**, 309, 111956. [Google Scholar] [CrossRef] - Kumar, V.; Lee, D.-J.; Lee, J.-Y. Studies of RTV silicone rubber nanocomposites based on graphitic nanofillers. Polym. Test.
**2016**, 56, 369–378. [Google Scholar] [CrossRef] - Olabi, A.; Abdelkareem, M.A.; Wilberforce, T.; Sayed, E.T. Application of graphene in energy storage device—A review. Renew. Sustain. Energy Rev.
**2021**, 135, 110026. [Google Scholar] [CrossRef] - Raccichini, R.; Varzi, A.; Passerini, S.; Scrosati, B. The role of graphene for electrochemical energy storage. Nat. Mater.
**2015**, 14, 271–279. [Google Scholar] [CrossRef] - Lu, H.; Yao, Y.; Huang, W.M.; Leng, J.; Hui, D. Significantly improving infrared light-induced shape recovery behavior of shape memory polymeric nanocomposite via a synergistic effect of carbon nanotube and boron nitride. Compos. Part B Eng.
**2014**, 62, 256–261. [Google Scholar] [CrossRef] - Lu, H.; Huang, W.M. Synergistic effect of self-assembled carboxylic acid-functionalized carbon nanotubes and carbon fiber for improved electro-activated polymeric shape-memory nanocomposite. Appl. Phys. Lett.
**2013**, 102, 231910. [Google Scholar] [CrossRef] - Barakzehi, M.; Montazer, M.; Sharif, F.; Norby, T.; Chatzitakis, A. A textile-based wearable supercapacitor using reduced graphene oxide/polypyrrole composite. Electrochim. Acta
**2019**, 305, 187–196. [Google Scholar] [CrossRef] - Bora, C.; Sharma, J.; Dolui, S. Polypyrrole/sulfonated graphene composite as electrode material for supercapacitor. J. Phys. Chem. C
**2014**, 118, 29688–29694. [Google Scholar] [CrossRef] - De Oliveira, H.P.; Sydlik, S.A.; Swager, T.M. Supercapacitors from free-standing polypyrrole/graphene nanocomposites. J. Phys. Chem. C
**2013**, 117, 10270–10276. [Google Scholar] [CrossRef] [Green Version] - Ding, X.; Zhao, Y.; Hu, C.; Hu, Y.; Dong, Z.; Chen, N.; Zhang, Z.; Qu, L. Spinning fabrication of graphene/polypyrrole composite fibers for all-solid-state, flexible fibriform supercapacitors. J. Mater. Chem. A
**2014**, 2, 12355–12360. [Google Scholar] [CrossRef] - Ghosh, D.; Giri, S.; Sahoo, S.; Das, C.K. In situ synthesis of graphene/amine-modified graphene, polypyrrole composites in presence of SrTiO
_{3}for supercapacitor applications. Polym. Technol. Eng.**2013**, 52, 213–220. [Google Scholar] [CrossRef] - Shu, K.; Wang, C.; Zhao, C.; Ge, Y.; Wallace, G.G. A free-standing graphene-polypyrrole hybrid paper via electropolymerization with an enhanced areal capacitance. Electrochim. Acta
**2016**, 212, 561–571. [Google Scholar] [CrossRef] [Green Version] - Zuo, X.; Zhang, Y.; Si, L.; Zhou, B.; Zhao, B.; Zhu, L.; Jiang, X. One-step electrochemical preparation of sulfonated graphene/polypyrrole composite and its application to supercapacitor. J. Alloys Compd.
**2016**, 688, 140–148. [Google Scholar] [CrossRef] - Zeng, X.; Yang, J.; Yuan, W. Preparation of a poly(methyl methacrylate)-reduced graphene oxide composite with enhanced properties by a solution blending method. Eur. Polym. J.
**2012**, 48, 1674–1682. [Google Scholar] [CrossRef] - Zhang, M.; Li, Y.; Su, Z.; Wei, G. Recent advances in the synthesis and applications of graphene—Polymer nanocomposites. Polym. Chem.
**2015**, 6, 6107–6124. [Google Scholar] [CrossRef] - Lago, E.; Toth, P.S.; Pugliese, G.; Pellegrini, V.; Bonaccorso, F. Solution blending preparation of polycarbonate/graphene composite: Boosting the mechanical and electrical properties. RSC Adv.
**2016**, 6, 97931–97940. [Google Scholar] [CrossRef] [Green Version] - Ajayan, P.M.; Stephan, O.; Colliex, C.; Trauth, D. Aligned carbon nanotube arrays formed by cutting a polymer resin—Nanotube composite. Science
**1994**, 265, 1212–1214. [Google Scholar] [CrossRef] [PubMed] - Lu, H.; Liang, F.; Gou, J. Nanopaper enabled shape-memory nanocomposite with vertically aligned nickel nanostrand: Controlled synthesis and electrical actuation. Soft Matter
**2011**, 7, 7416–7423. [Google Scholar] [CrossRef] - Folorunso, O.; Hamam, Y.; Sadiku, R.; Ray, S.S.; Joseph, A.G. Parametric Analysis of Electrical Conductivity of Polymer-Composites. Polymers
**2019**, 11, 1250. [Google Scholar] [CrossRef] [Green Version] - Taherian, R. Developments and modeling of electrical conductivity in composites. In Electrical Conductivity in Polymer-Based Composites: Experiments, Modelling and Applications; Elsevier Applied Science Publishers: Waltham, MA, USA, 2019; pp. 297–363. [Google Scholar] [CrossRef]
- Clingerman, M.L. Development and Modelling of Electrically Conductive Composite Materials; Michigan Technological University: Houghton, MI, USA, 2001. [Google Scholar]
- Weber, M.; Kamal, M.R. Estimation of the volume resistivity of electrically conductive composites. Polym. Compos.
**1997**, 18, 711–725. [Google Scholar] [CrossRef] - Taherian, R. Development of an equation to model electrical conductivity of polymer-based carbon nanocomposites. ECS J. Solid State Sci. Technol.
**2014**, 3, M26–M38. [Google Scholar] [CrossRef] - Folorunso, O.; Hamam, Y.; Sadiku, R.; Ray, S.S.; Adekoya, G.J. Electrical Resistance control model for polypyrrole-graphene nanocomposite: Energy storage applications. Mater. Today Commun.
**2020**, 26, 101699. [Google Scholar] [CrossRef] - Folorunso, O.; Hamam, Y.; Sadiku, R.; Ray, S.S.; Adekoya, G.J. Statistical characterization and simulation of graphene-loaded polypyrrole composite electrical conductivity. J. Mater. Res. Technol.
**2020**, 9, 15788–15801. [Google Scholar] [CrossRef] - Gong, S.; Zhu, Z.H.; Haddad, E.I. Modeling electrical conductivity of nanocomposites by considering carbon nanotube deformation at nanotube junctions. J. Appl. Phys.
**2013**, 114, 074303. [Google Scholar] [CrossRef] - Li, C.; Thostenson, E.T.; Chou, T.-W. Dominant role of tunneling resistance in the electrical conductivity of carbon nanotube–based composites. Appl. Phys. Lett.
**2007**, 91, 223114. [Google Scholar] [CrossRef] - Kumar, V.; Lee, J.-Y.; Lee, D.-J. Synergistic effects of hybrid carbon nanomaterials in room-temperature-vulcanized silicone rubber. Polym. Int.
**2017**, 66, 450–458. [Google Scholar] [CrossRef] - Kirkpatrick, S. Percolation and conduction. Rev. Mod. Phys.
**1973**, 45, 574–588. [Google Scholar] [CrossRef] - Clingerman, M.L.; King, J.A.; Schulz, K.H.; Meyers, J.D. Evaluation of electrical conductivity models for conductive polymer composites. J. Appl. Polym. Sci.
**2001**, 83, 1341–1356. [Google Scholar] [CrossRef] - McCullough, R. Generalized combining rules for predicting transport properties of composite materials. Compos. Sci. Technol.
**1985**, 22, 3–21. [Google Scholar] [CrossRef] - Vahidi, K.; Jalili, Y.S. Modification of surface energy and electrical and thermal properties of spherical polypyrrole nanoparticles synthesized by CTAB for potential application as a conductive ink. J. Theor. Appl. Phys.
**2013**, 7, 1–9. [Google Scholar] [CrossRef] [Green Version] - Sánchez-González, J.; Macías-García, A.; Alexandre-Franco, M.; Gómez-Serrano, V. Electrical conductivity of carbon blacks under compression. Carbon
**2005**, 43, 741–747. [Google Scholar] [CrossRef] - Scriba, M.R. Synthesis and Characterisation of Doped Silicon Nanoparticles by Hot Wire Thermal Catalytic and Spark Pyrolysis; University of Cape Town: Cape Town, South Africa, 2010. [Google Scholar]
- Braun, H.; Euler, K.-J.; Herger, P. Electronic conductivity of lead dioxide powder: Separation of core and surface resistance of the particles. J. Appl. Electrochem.
**1980**, 10, 441–448. [Google Scholar] [CrossRef] - Mamunya, Y.; Zois, H.; Apekis, L.; Lebedev, E. Influence of pressure on the electrical conductivity of metal powders used as fillers in polymer composites. Powder Technol.
**2004**, 140, 49–55. [Google Scholar] [CrossRef] - Kim, S.Y.; Noh, Y.J.; Yu, J. Prediction and experimental validation of electrical percolation by applying a modified micromechanics model considering multiple heterogeneous inclusions. Compos. Sci. Technol.
**2015**, 106, 156–162. [Google Scholar] [CrossRef] - Wang, L.; Liu, F.; Jin, C.; Zhang, T.; Yin, Q. Preparation of polypyrrole/graphene nanosheets composites with enhanced thermoelectric properties. RSC Adv.
**2014**, 4, 46187–46193. [Google Scholar] [CrossRef] - Ansari, R. Thermal Studies of Conducting Electroactive Polymers. Ph.D. Thesis, University of Wollongong, Wollongong, NSW, Australia, 1995. [Google Scholar]
- Ruhi, G.; Bhandari, H.; Dhawan, S. Corrosion resistant polypyrrole/flyash composite coatings designed for mild steel substrate. Am. J. Polym. Sci.
**2015**, 5, 18–27. [Google Scholar] - Ningaraju, S.; Ravikumar, H. Ionic and electronic transport in PSF/NiO and PSF/TiO
_{2}polymer nanocomposites: A positron lifetime study. Solid State Ion.**2017**, 310, 81–94. [Google Scholar] [CrossRef] - Tuncer, E. The glass transition and DC conductivity in highly filled composites. Mater. Res. Express
**2017**, 4, 045905. [Google Scholar] [CrossRef] - Mavinakuli, P.; Wei, S.; Wang, Q.; Karki, A.B.; Dhage, S.; Wang, Z.; Young, D.P.; Guo, Z. Polypyrrole/silicon carbide nanocomposites with tunable electrical conductivity. J. Phys. Chem. C
**2010**, 114, 3874–3882. [Google Scholar] [CrossRef] - Canales, J.; Muñoz, M.E.; Fernández, M.; Santamaría, A. Rheology, electrical conductivity and crystallinity of a polyurethane/graphene composite: Implications for its use as a hot-melt adhesive. Compos. Part A Appl. Sci. Manuf.
**2016**, 84, 9–16. [Google Scholar] [CrossRef] - Gültner, M.; Häußler, L.; Pötschke, P. Influence of matrix crystallinity on electrical percolation of multiwalled carbon nanotubes in polypropylene. In Proceedings of the 32nd International Conference of the Polymer Processing Society, Lyon, France, 25–29 July 2016; p. 030022. [Google Scholar]
- Feng, X.; Li, R.; Yan, Z.; Liu, X.; Chen, R.; Ma, Y.; Li, X.; Fan, Q.; Huang, W. Preparation of graphene/polypyrrole composite film via electrodeposition for supercapacitors. IEEE Trans. Nanotechnol.
**2012**, 11, 1080–1086. [Google Scholar] [CrossRef] - Guadagno, L.; Vietri, U.; Raimondo, M.; Vertuccio, L.; O’ Barra, G.M.; De Vivo, B.; Lamberti, P.; Spinelli, G.; Tucci, V.; De Nicola, F.; et al. Correlation between electrical conductivity and manufacturing processes of nanofilled carbon fiber reinforced composites. Compos. Part B Eng.
**2015**, 80, 7–14. [Google Scholar] [CrossRef] - Liu, Y.; Zhang, Y.; Ma, G.; Wang, Z.; Liu, K.; Liu, H. Ethylene glycol reduced graphene oxide/polypyrrole composite for supercapacitor. Electrochim. Acta
**2013**, 88, 519–525. [Google Scholar] [CrossRef] - Stankovich, S.; Dikin, D.A.; Dommett, G.H.B.; Kohlhaas, K.M.; Zimney, E.J.; Stach, E.A.; Piner, R.D.; Nguyen, S.T.; Ruoff, R.S. Graphene-based composite materials. Nat. Cell Biol.
**2006**, 442, 282–286. [Google Scholar] [CrossRef] [PubMed]

**Figure 3.**SEM graphs of (

**a**) $\mathrm{HGPPy}.{\mathrm{CB}}_{20\%}$ 1:3 (

**b**) $\mathrm{HGPPy}.{\mathrm{CB}}_{20\%}$ 3:7 (

**c**) $\mathrm{HGPPy}.{\mathrm{CB}}_{20\%}$ 7:13.

**Figure 4.**Temperature of analysis of Gr and $\mathrm{PPy}.{\mathrm{CB}}_{20\%}$. W-PPy.CB

_{20%}and W-Gr are the percentage weight curves. D-PPy.CB

_{20%}and D-Gr are the derivatives curves.

**Figure 5.**The hybrids temperature analysis: (

**a**–

**d**) percentage weight curve of $\mathrm{HGPPy}.{\mathrm{CB}}_{20\%}$ 1:3, $\mathrm{HGPPy}.{\mathrm{CB}}_{20\%}3:7$, $\mathrm{HGPPy}.{\mathrm{CB}}_{20\%}7:13$, $\mathrm{PPy}.{\mathrm{CB}}_{20\%}$ and (

**e**–

**h**) derivatives curve of $\mathrm{PPy}.{\mathrm{CB}}_{20\%}$, $\mathrm{HGPPy}.{\mathrm{CB}}_{20\%}$ 1:3, $\mathrm{HGPPy}.{\mathrm{CB}}_{20\%}3:7$, $\mathrm{HGPPy}.{\mathrm{CB}}_{20\%}7:13$.

**Figure 6.**DSC thermograms for $\mathrm{PPy}.{\mathrm{CB}}_{20\%}$ and $\mathrm{HGPPy}.{\mathrm{CB}}_{20\%}$ (

**a**) $\mathrm{PPy}.{\mathrm{CB}}_{20\%}$ (

**b**) $\mathrm{HGPPy}.{\mathrm{CB}}_{20\%}$ 1:3 (

**c**) $\mathrm{HGPPy}.{\mathrm{CB}}_{20\%}$ 3:7 (

**d**) $\mathrm{HGPPy}.{\mathrm{CB}}_{20\%}$ 7:13.

Models | Parameter | Parameter Value | Standard Error | Per Unit Standard Error | R^{2} | R^{2}-Adj. |
---|---|---|---|---|---|---|

Weber | ${\beta}_{1}$ | 2.8504 | 0.1015 | 0.0453 | 0.923 | 0.907 |

Models | Parameters | Parameters Values | Standard Error | Per Unit Standard Error | R^{2} | R^{2}-Adj. |
---|---|---|---|---|---|---|

Clingerman | ${\alpha}_{1}$ | 1720.8 | 255.68 | 0.1486 | 0.964 | 0.927 |

${\alpha}_{2}$ | 3.8000 | 0.5413 | 0.1426 | |||

${\alpha}_{3}$ | 0.3000 | 0.0480 | 0.1594 | |||

${\alpha}_{4}$ | 1.1100 | 0.0132 | 0.0119 |

Models | Parameters | Parameters Values | Standard Error | Per Unit Standard Error | R^{2} | R^{2}-Adj. |
---|---|---|---|---|---|---|

Taherian | ${\gamma}_{1}{\sigma}_{f}$ | 2278 | 408 | 0.1789 | 0.967 | 0.950 |

${\gamma}_{2}$ | 10.54 | 2.96 | 0.2810 | |||

${\gamma}_{3}$ | 0.19 | 0.04 | 0.2270 |

Publisher’s Note: MDPI stays neutral with regard to jurisdictional claims in published maps and institutional affiliations. |

© 2021 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).

## Share and Cite

**MDPI and ACS Style**

Folorunso, O.; Hamam, Y.; Sadiku, R.; Ray, S.S.; Kumar, N.
Investigation and Modeling of the Electrical Conductivity of Graphene Nanoplatelets-Loaded Doped-Polypyrrole. *Polymers* **2021**, *13*, 1034.
https://doi.org/10.3390/polym13071034

**AMA Style**

Folorunso O, Hamam Y, Sadiku R, Ray SS, Kumar N.
Investigation and Modeling of the Electrical Conductivity of Graphene Nanoplatelets-Loaded Doped-Polypyrrole. *Polymers*. 2021; 13(7):1034.
https://doi.org/10.3390/polym13071034

**Chicago/Turabian Style**

Folorunso, Oladipo, Yskandar Hamam, Rotimi Sadiku, Suprakas Sinha Ray, and Neeraj Kumar.
2021. "Investigation and Modeling of the Electrical Conductivity of Graphene Nanoplatelets-Loaded Doped-Polypyrrole" *Polymers* 13, no. 7: 1034.
https://doi.org/10.3390/polym13071034